Synthesis and Visible-Light Photocatalytic Property of Bi2WO6Hierarchical Octahedron-Like Structures
© to the authors 2008
Received: 8 August 2008
Accepted: 2 September 2008
Published: 19 September 2008
Skip to main content
© to the authors 2008
Received: 8 August 2008
Accepted: 2 September 2008
Published: 19 September 2008
A novel octahedron-like hierarchical structure of Bi2WO6has been fabricated by a facile hydrothermal method in high quantity. XRD, SEM, TEM, and HRTEM were used to characterize the product. The results indicated that this kind of Bi2WO6crystals had an average size of ~4 μm, constructed by quasi-square single-crystal nanosheets assembled in a special fashion. The formation of octahedron-like hierarchical structure of Bi2WO6depended crucially on the pH value of the precursor suspensions. The photocatalytic activity of the hierarchical Bi2WO6structures toward RhB degradation under visible light was investigated, and it was found to be significantly better than that of the sample fabricated by SSR. The better photocatalytic property should be strongly associated with the high specific surface area and the abundant pore structure of the hierarchical octahedron-like Bi2WO6.
Since the discovery of photoelectrochemical water splitting at a semiconductor surface in 1972, great progress has been made in the research of photocatalytic degradation of organic pollutants for solving environmental problems that confront mankind today. Photocatalysis has many advantages over other treatment methods, for instance, the use of the environmentally friendly oxidant O2, the easy reaction performed at room temperature, and oxidation of the organic compounds even at low concentrations [1–3]. Much work on photocatalysis in the past decade has focused on TiO2 for its excellent behaviors in the oxidative degradation of many organic compounds under UV irradiation [4–10]. However, the relatively wide bandgap of 3.2 eV limits its efficient utilization because the UV range is only about 4% of the solar spectrum. In view of the largest proportion of the solar spectrum and artificial light sources, the development of photocatalysts with high activity under a wide range of visible-light irradiation is highly desirable.
There are generally two ways to exploit the photocatalysts responsive to visible-light irradiation: the first involves the modification of TiO2, and the second is the development of a new photocatalytic material. The former has been extensively investigated by doping with metallic or nonmetallic elements such as V and Cr [11–13] or N [14–18], S [19–21], C [22–24], to gain visible-light response. In contrast, there have been only a few reports on the development of new photocatalyst materials [25–28].
Bi2WO6, the simplest member in the Aurivillius family and a potential visible-light photocatalyst, was first studied by Kudo and Hijii , Zou’s and co-workers  groups. Their works revealed that Bi2WO6 could perform as an excellent photocatalytic and solar energy transfer material. Photocatalytic activities for O2 evolution/water splitting and the degradation of the CHCl3 and CH3CHO under visible-light irradiation were discussed in detail. Encouraged by this progress, various Bi2WO6 nanostructures including nanoplates and nanoparticles synthesized by hydrothermal method and their enhanced visible-light-driven photocatalytic activity such as photodegradation of rhodamine B(RhB) were reported subsequently [31–35]. On the other hand, spherical superstructures constructed by nano-substructures have been attracting much interest due to their micro/nanostructure and the distinguished physical/chemical properties [36–41]. Large specific surface area and porous structures induced by the hierarchical configuration may improve the contact/interaction between materials and the organic compounds, and thus lead to better photocatalytic performance. As a result, several hierarchical three-dimensional (3D) structures of Bi2WO6 [42–44] were also fabricated in the past 2 years.
In a previous work, we fabricated uniform Bi2WO6 microspheres governed by a layer-by-layer growth mechanism . We report herein, for the first time, another novel octahedron-like hierarchical structure of Bi2WO6 consisting of quasi-square plates joined vertically, and demonstrate its improved visible-light photocatalytic activity in the degradation of RhB as compared to that of the Bi2WO6 synthesized by solid-state reaction (SSR). The results indicate that the pH value of precursor suspensions has impact on the morphology of as-prepared products. In addition, the photocatalyst of octahedron-like hierarchically structured Bi2WO6 dispersed in alkaline solutions is found to show significantly better photocatalytic ability. Our work will help to develop promising nanostructured photocatalysts that can be more easily separated and recycled.
In a typical procedure, Bi(NO3)3 · 5H2O (2 mmol) was added to 20 mL 1 M HNO3 to form a clear solution under stirring for 30 min at room temperature. Afterward, 50 mL solution of dissolved 1 mmol Na2WO4 · 2H2O and 0.1 g of PVP was added into the above solution, and a lot of white precipitate appeared quickly. The pH value of the suspension was adjusted to 7 by adding NH3 · H2O. After constant stirring for another 30 min, the mixture was finally transferred into a 100 mL Teflon-lined autoclave and filled with deionized water up to 80% of the total volume. The autoclave was sealed, maintained at 180 °C for 12 h, and cooled to room temperature naturally. The white precipitate was collected and rinsed several times with distilled water and absolute ethanol, respectively. Then, the sample was dried in a vacuum at 60 °C. For comparison purpose, we also fabricated Bi2WO6 by traditional SSR according to Ref.  and dispersed nanoplate sample without using PVP.
The phase purity of the as-prepared products was determined by X-ray diffraction (XRD Y-2000) with Cu Kα radiation (λ = 1.5418 Å) at a scan rate of 0.04°s−1. The morphology of the as-prepared product was characterized by field-emission scanning electron microscopy (FESEM, JEOL, JSM-6700F). Transmission electron microscopy (TEM) was taken with a FEI H-800 transmission electron microscope at an acceleration voltage of 200 kV to further investigate the morphology and structure of Bi2WO6structures. High-resolution transmission electron microscope (HRTEM) images and selected area electron diffraction (SAED) patterns were performed on a JEOL-2010 transmission electron microscope. Room-temperature UV–Vis absorption spectrum was recorded on a UV-1700 spectrophotometer in the wavelength range of 400–800 nm.
Photocatalytic activity was evaluated by the degradation of RhB under visible-light irradiation using a 300 W Xe lamp with a cutoff filter (λ > 400 nm). The reaction cell was placed in a sealed black box, the top of which was open, and the cutoff filter was set on the window face of the reaction cell to ensure the desired irradiation condition. In each experiment, photocatalyst powders (0.5 g/L) were added into RhB solution (1 × 10−5 M, 500 mL). Before illumination, the suspensions were magnetically stirred in the dark for 60 min to ensure the establishment of an adsorption–desorption equilibrium between photocatalyst powders and RhB. At given time intervals, 3 mL suspensions were sampled and centrifuged to remove photocatalyst powders. The filtrates were analyzed by recording the variations of the absorption-band maximum (553 nm) in the UV–Vis spectrum of RhB.
The X-ray powder diffraction pattern of the product (Fig. 2b) can be indexed as pure orthorhombic Bi2WO6, consistent with the reported data (JCPDS card No. 73-1126, a = 5.457 Å, b = 5.436 Å, c = 16.42 Å). Compared with the standard pattern inserted in Fig. 2b, the intensity ratio of the (200)/(020) peak to the (113) peak increases to 0.61 in the present case, apparently larger than the standard value 0.185, which demonstrates the faster growth of Bi2WO6 crystal along the (200)/(020) plane .
As we know, the pH value of the precursor suspension has a strong effect on the hydrolysis of Bi3+ , which determines the rates of Bi2WO6 nucleation and crystal growth. At low pH value (below 1), the H+ concentration is much higher than OH− ion concentration, restraining the hydrolysis of the Bi3+; thus the nucleation rate of Bi2WO6 has absolute priority over that of crystal growth. As a result, the product is in the form of a microspherical particle constructed by nanoplate subunits according to thermodynamic stability condition (Fig. 4a). The formation of plate-like substructures results from the intrinsic anisotropic layered structure of Bi2WO6 [31, 44]. At high pH value (about 10), the rapid hydrolysis of Bi3+ decreases the quantity of Bi2WO6 nuclei and then the pre-formed seeds have enough resource to contiguously grow and finally form Bi2WO6 microplates. In the moderate pH value (~7), the formation of Bi2WO6 nanoplates with appropriate quantity is accompanied by a unique self-assembly process, giving rise to octahedron-like hierarchical structures composed of both parallel and vertical plates. For the assembly of such unique microstructures, the function of PVP and the crystal structure of Bi2WO6 material should be considered. Previously, PVP was successfully applied as an important surfactant for the synthesis of various hierarchical nanostructures. In the present work, it was believed that the selective adsorption of PVP on some crystallographic planes of Bi2WO6 subunits (small nanoplates) can take place at the initial growth stage. This would help to generate many uniform subunits. As growth time proceeded, the initially formed small plates assembled in an edge-to-edge way with the gradual enlargement of the 2D surfaces. This assembly process greatly lowered the interfacial energy  and was facilitated by the square shape of the subunits, which resulted from the crystal structure of Bi2WO6. A subsequent layer-by-layer growth of the large nanoplates gave many parallel square plates. Since the formation of parallel plates occurred simultaneously in three dimensions, we could finally observe three groups of parallel square plates cross-linked with (and vertical to) each other, forming octahedron-like structures.
It is noteworthy that our octahedron-like hierarchical Bi2WO6shows significantly improved photocatalytic activity in comparison with the sample obtained by SSR. As seen from inset of Fig. 6, only 31% of the RhB can be removed after 6-h irradiation when SSR-produced sample is used as the photocatalyst. The reasons accounting for the better photocatalytic activity of our Bi2WO6structures can be explained as follows: (1) photocatalytic process is mainly related to the adsorption and desorption of molecules on the surface of the catalyst. The relatively high specific surface area of the 3D hierarchical structure and a large number of pores in the structure allow more efficient transport of the organic molecules to the active reaction sites, hence enhancing the efficiency of photocatalysis. (2) The high surface-to-volume ratios of nanoplate subunits are beneficial to the separation/transfer of electrons and holes. Due to the laminar structure, holes generated inside the crystals have greater opportunity to transfer to the surface and act with the RhB. Indeed, as shown in the inset of Fig. 6, nanoplates exhibit much better catalytic ability than SSR sample. (3) Porous appearance in the octahedron-like hierarchical structures may also enhance visible-light transmission and utilization. It should be further pointed out that the 3D hierarchical structures can be readily dispersed due to the micrometer size, avoiding the unwanted aggregations (this exists in nanoplate sample) during the photocatalytic process. Also, the larger size will facilitate the separation and recycling of photocatalysts, which is very important for environmental application.
In this paper, we report the hydrothermal synthesis of a novel hierarchical octahedron-like structure of Bi2WO6, which has an average size of ~4 μm and consists of many quasi-square nanosheets. The effect of pH value of the precursor suspensions on the formation of octahedron-like Bi2WO6crystals is discussed. Importantly, as a potential visible-light photocatalyst, our octahedron-like Bi2WO6exhibits much better activity for the photodegradation of RhB as compared to the photocatalyst product fabricated by SSR.